Dr Chris Corti is a technologist with over 38yrs experience developing and exploiting
technology in the precious metals industry. He worked with Johnson Matthey Plc and
World Gold Council before setting up his own technology consultancy in 2009. He studied
metallurgy at University and has worked in the energy industry in the UK and Switzerland
before moving into the precious metal industry. He has published widely and presented
on jewellery topics many times at the Jewellery Technology Forum and the Santa Fe
Heat treatment of precious metal jewellery alloys is often referred to in the literature but
many practitioners do not have a clear understanding of what this term means and its
importance to the jewellery industry. It is a term often used by metallurgists to describe
a range of thermal processes designed to manipulate properties of engineering and
decorative alloys to meet requirements. Many will be familiar with heating and quenching of
steel to harden it, whilst age-hardening of steels and aluminium alloys is an example of a
two-stage treatment that is widely used to confer additional strength.
Many treatments involve heating of the alloys to specific temperatures for specified periods
of time and then cooling at a defined rate that may be rapid or slow. In jewellery, annealing
of precious metal alloys is often undertaken to soften cold-worked material to enable further
working without cracking or fracture. But other types of annealing are also carried out,
for example to stress relieve alloy items to prevent stress corrosion cracking or to age-
harden them. In investment casting, the burning out of casting moulds (‘flasks’) requires a
defined temperature and time cycle to enable good castings to be achieved. This is also an
example of a heat treatment.
Whilst annealing and age-hardening of jewellery metals has been featured in previous JTF
presentations, the ‘whys’ and ‘wherefores’ of such treatments have not, perhaps, been
fully explained. There are several types of annealing treatments in use, each with different
objectives. This presentation focuses on heat treatments used in the jewellery industry and
attempts to explain the underlying principles involved. Examples of heat treatments of base
metal alloys are also included to demonstrate that such treatments are universal.
2Jewelry Technology Forum 2017
“Improving the Properties of Precious Metals by Heat Treatment”
A participant at a recent jewellery technology symposium made a remark, following my Basic Metallurgy presentation1, “I don’t
understand what ‘heat treatment’ is!”. It made me think whether I have missed something important in this series of presentations
made at the Santa Fe Symposia. Actually, it is mostly covered but, perhaps, was not fully clear and explained as a discrete topic. This
presentation is made to repair this omission.
So what does the term ‘Heat treatment’ mean and what does it cover? Basically, it is a broad term to cover any treatment of a metal
or alloy that involves heating it for a period of time to change some aspect of its properties. To put it more technically, heat treatment
is a term often used by metallurgists to describe a range of thermal processes designed to manipulate properties of engineering and
decorative alloys to meet requirements. Heating and quenching of steel to harden it is one example that results from a phase change
from austenite to martensite, a phase change that involves the shearing of atoms within the crystals (grains). The crystal structure
changes from face-centered cubic (FCC) to face-centered tetragonal (FCT). Age-hardening (or precipitation hardening) of steels and
aluminum alloys are examples of a two-stage treatment that is widely used to confer additional strength, often at the expense of some
ductility. Hardening of die steels for forging and stamping operations is one example with which many of us will be familiar. We can
use this mechanism for some jewellery alloys too, as we shall see later.
Many treatments involve heating of the alloys to specific temperatures for specified periods of time and then cooling at a defined
rate that may be rapid or slow. In jewellery, annealing of precious metal alloys is often undertaken to soften cold-worked material to
enable further working without cracking or fracture. But other types of annealing are also carried out: for example, to stress relieve
alloy items to prevent stress corrosion cracking or to age-harden them. To cite a non-metallic example: in investment casting, the
burning out of casting molds (‘flasks’) requires a defined temperature and time cycle to enable good quality moulds (and hence
castings) to be achieved. This is also a heat treatment of the mould!
Whilst annealing and age-hardening of jewellery metals has been discussed in previous ‘Basic Metallurgy’ presentations, the ‘whys’
and ‘wherefores’ of such treatments have not, perhaps, been fully explained. There are several types of annealing treatments in use,
for example, each with different objectives. This presentation focuses on heat treatments used in the jewellery industry and attempts
to explain the underlying principles involved. I will also give some other examples for base metal alloys used in the engineering
TYPES OF HEAT TREATMENT
There are many types of heat treatment in use in the metallurgical industry. Some are not used for precious metals used in the
jewellery industry, for example, and some may involve controlled atmospheres to prevent oxidation or to diffuse an element into the
component surface or, conversely, out of the alloy. Carburizing of plain carbon steels to form a hard surface layer to give improved
wear resistance is an example of diffusing carbon into the steel surface whilst Sage in 2010 gave us an example of diffusing oxygen
out of the surface as a way of removing firestain from silver2. Diffusion bonding of different alloys together requires both temperature
and pressure to achieve metallurgical bonding and is used to make materials for mokume gane3,4. This is an example of a diffusion
heat treatment. Temperature and pressure are also used in Hot Isostatic Pressing to remove casting defects24. The point I make here
is that the term ‘Heat treatment’ is a general term and is a process carried out for a variety of reasons.
3Jewelry Technology Forum 2017
Some of the types of heat treatment we use in our industry include:
1. Softening treatments (usually called ‘annealing’) to relieve internal stress and recover ductility. This includes full annealing, to
recrystallize the microstructure, and stress-relief annealing to inhibit stress corrosion cracking in the carat golds. How we cool the
alloy down after the heating cycle can be important too. Solution annealing and quenching in water is another that we use to get
a softer condition that results from dissolving second phases back into the matrix phase or, simply, to obtain a higher temperature
matrix phase. This is also the first stage of age-hardening treatments.
2. Hardening treatments to get additional strength by precipitation of finely-sized second phases within the microstructure. These
second phases may be other solid solutions of the main alloying metal, but often these may be intermetallic phases, comprising two
or metals in fixed proportions to produce a metal compound. In aluminum alloys, these may be aluminum-copper or -magnesium
based compounds. We can take this approach to harden certain alloys of platinum, gold and even silver. In steels, we often precipitate
carbides and nitrides in the microstructure to harden them. For silver-based electrical contact materials, we internally oxidize a silver-
cadmium alloy by heating in an oxidizing atmosphere to form a dispersion of hard cadmium oxide particles within the structure. This
hardens the alloy and improves erosion/wear during electrical switching operations.
3. Diffusion treatments are used for various reasons. Firstly, to homogenize alloy microstructures in terms of chemical composition,
i.e. to remove segregation from casting. This involves heating to high temperatures, but below the solidus, for a long time. Another
reason that we have already mentioned is to bond dissimilar alloys together. This also involves high temperatures for a period of
time but additionally under pressure. The aim is to encourage atoms of each alloy to diffuse across the boundary into the other alloy,
forming a strong metallurgical bond. Such techniques are also used for diffusion soldering1. We have also mentioned earlier the use
of surface diffusion treatments to diffuse elements into the surface or to remove unwanted elements out of the surface.
4. Decorative treatments. I include here thermal treatments to oxidize the surface to produce decorative effects, as is used for some
of the unusual colored golds5 and to produce surface effects such as found with ‘Spangold’ alloys6 which are based on a martensitic
phase transformation. I do not intend to say more on these treatments in this presentation today.
Annealing treatments are carried out to soften a cold-worked alloy, i.e. to restore some measure of ductility that has been lost due
to the prior working. This may be to enable further working to be carried out without risk of cracking or fracture, or simply because
a softer, stress-relieved condition is preferred. The term ‘working’ refers to mechanically deforming an alloy to change its shape.
This may also result in the breakdown of a coarse microstructure. Working may be carried out hot or